Supporting InformationELECTRONIC SUPPLEMENTARY INFORMATION
Synthesis and Dye Sensitized Solar Cell Applications of Bodipy
Derivatives with Bis- dimethylfluorenyl Amino Donor Groups
Yusuf Çakmak, *a Safacan Kolemen,a Muhammed Buyuktemiz, b Yavuz
Dede, b Sule Erten-Ela,*c aDepartment of Chemistry, Bilkent
University, Ankara, 06800, Turkey b Department of Chemistry,
Faculty of Science, Gazi University, Teknikokullar, Ankara 06500,
Turkey cInstitute of Solar Energy, Ege University, Izmir, 35100,
Turkey. TEL: 0090 232 3111231; E-mail: [email protected]
Electronic structure analysis of dyes TB6 and TB7 were performed
with Density Functional Theory3-6 employing the
B3LYP5-11, functional and Stevens-Basch-Krauss split valence
efective core potentials (ECP) CEP-31G.13 This level of
theory was previously shown to yield reasonable results for similar
systems.14-15 For both cases, symmetry is turned off and
unrestricted DFT formalism is followed. Spin contaminations of the
Kohn Sham wave functions were checked and found to
be negligible in all cases. Harmonic vibrational frequency
calculations ensured that Hessian matrix does not contain any
negative eigenvalue, i.e. all reported geometries correspond to
minimum points on the potential energy surface. Excitations
were studied with the TD-DFT formalism. The Polarizable Continuum
Model (PCM) is used to model the dielectric medium
of methanol solvent. Computations were carried out using Gaussian
0916. Molecular orbitals are plotted using 0.3 iso-value.
The construction of the dye sensitized solar cell device requires
first cleaning of the fluorine doped tin oxide (FTO)
coated glass substrates in acetone and isopropanol by using an
ultrasonic bath. FTO (SnO2:F, Pilkington TEC-15;
Rsheet:15O/&), electrically conductive oxide-coated glasses
were used as transparent electrodes. TiO2 electrodes consist
an adsorbent mesoporous layer with 20 nm anatase TiO2 particle size
in 7 mm thicknesses and a second light scattering layer
with 400 nm anatase TiO2 particle size of 5 mm thicknesses. Dye
solutions were prepared in chlorobenzene-methanol (1:1)
mixture with a concentration of 0.5 mM BODIPY. TiO2-coated
electrodes, after sintering at 4500C for 30 min and cooling
1000C, were kept overnight in BODIPY solutions for adsorption.
BODIPY adsorbed TiO2-coated glasses were washed with
pure chlorobenzene and dried in vacuo. Platinized FTO glasses were
used as counter electrode. Platinization of counter
electrodes were done by coating of FTO glasses with 1% solution of
hydrogen hexachloroplatinate (Aldrich) in 2-propanol
and annealing at 4000C for 30 min. Cells were prepared in sandwich
geometry. Surlyn-1702 (DuPont) frame was used as a
spacer and a thermoplastic sealant between the two electrodes.
Cells prepared in this way were then sealed by heating at
1000C. Electrolyte was filled into the space created by Surlyn-1702
between the electrodes under vacuum using a small hole
pre-drilled on the counter electrode with the help of a diamond
drill. After filling the electrolyte, a small hole was sealed
again using a piece of Surlyn-1702 and a piece of cover glass. The
electrolyte consisted of 0.6M N-methyl-N-butyl-
imidazolium iodide (BMII) + 0.1 M LiI + 0.05 M I2 + 0.5 M
4-tert-butylpyridine (TBP) in acetonitrile/valeronitrile
v/v). Active areas of the cells were adjusted to 0.159 cm2 with a
special mask. Dye sensitized solar cells were characterized
by current-voltage (J −V ) measurement. All current-voltage
measurements (J −V ) were done under 100 mW/cm2 light
intensity and AM 1.5 conditions. 450 W Xenon light source (Oriel)
was used to give an irradiance of various intensities. The
spectral output of the lamp was matched in the region of 350–700 nm
with the aid of Schott K113 Tempax sunlight filter. J −
V data collection was made by using Keithley 2400 Source-Meter and
LabView data acquisition software. The incident
Electronic Supplementary Material (ESI) for New Journal of
Chemistry. This journal is © The Royal Society of Chemistry and the
Centre National de la Recherche Scientifique 2015
photon-to-current conversion efficiencies (IPCE) were taken in the
equipment of QE-R Enlitech. All of the dye scan
efficiently convert visible light to photocurrent in the region
from 300 nm to 700 nm.
Figure S2: 1H NMR Spectrum of TB5
Figure S3: 1H NMR and 13C Spectra of TB6
Figure S4: 1H NMR and 13C Spectra of TB7
CHARACTERIZATION OF DSSC
400 450 500 550 600 650 700 750 800 0
Figure S6. Incident photon to current conversion efficiencies as a
function of wavelength for the liquid electrolyte based
Figure S7. Scanning electron microscopy image (SEM) of TiO2
SEM images of TiO2 electrode was given in Figure S7. Both
sensitizers have been used to manufacture solar cell
devices to explore current-voltage characteristics using
7(transparent) + 5(scattering) m TiO2 transparent layers.
and characterization of double-layer TiO2 electrode are previously
described by Wang et al.16
Atomic Force Microscopy Images of the Films
Morphology of the films were observed by Atomic Force Microscopy
using Ambios AFM equipment. Atomic force
microscopy (AFM) is used to observe film surface morphology of TiO2
(a), TB5 on TiO2 (b), TB6 on TiO2 (c), TB7 on TiO2
(d). AFM images of films in noncontact mode are presented in Fig.
Figure S7. AFM images of mesoporous TiO2 (a), TB5 on TiO2 (b), TB6
on TiO2 (c), TB7 on TiO2 (d)
1 Kohn, W., Becke, A. D. & Parr, R. G. Density functional
theory of electronic structure. J. Phys. Chem. 100, 12974- 12980
2 Parr, R. G. & Yang, W. Density Functional Theory of Atoms and
Molecules. (Oxford University Press, 1989). 3 Becke, A. D.
Density-Functional Thermochemistry. 3. The Role of Exact Exchange.
J. Chem. Phys. 98, 5648-5652
(1993). 4 Becke, A. D. Density-Functional Exchange-Energy
Approximation With Correct Asymptotic-Behavior. Phys. Rev.
A 38, 3098-3100 (1988). 5 Lee, C. T., Yang, W. T. & Parr, R. G.
Development of the Colle-Salvetti Correlation-Energy Formula Into
Functional of the Electron-Density. Phys. Rev. B 37, 785-789
(1988). 6 Slater, J. C. Quantum Theory of Molecules and Solids,
Vol. 4: The Self-Consistent Field for Molecules and Solids.
(McGraw-Hill, 1974). 7 Vosko, S. H., Wilk, L. & Nusair, M.
Accurate Spin-Dependent Electron Liquid Correlation Energies for
Spin-Density Calculations - a Critical Analysis. Can. J. Phys. 58,
1200-1211 (1980). 8 Stephens, P. J., Devlin, F. J., Chabalowski, C.
F. & Frisch, M. J. Ab Initio Calculation of Vibrational
and Circular Dichroism Spectra Using Density Functional Force
Fields doi:10.1021/j100096a001. J. Phys. Chem. 98, 11623-11627
9 Hertwig, R. H. & Koch, W. On the parameterization of the
local correlation functional. What is Becke-3-LYP? Chem. Phys.
Lett. 268, 345-351 (1997).
10 Stevens, W. J., Basch, H. & Krauss, M. Compact Effective
Potentials and Efficient Shared-Exponent Basis-Sets for the 1st-Row
and 2nd-Row Atoms. J. Chem. Phys. 81, 6026-6033 (1984).
11 Cakmak, Y. et al. Designing Excited States: Theory-Guided Access
to Efficient Photosensitizers for Photodynamic Action. Angew. Chem.
Int. Ed. 50, 11937-11941 (2011).
12 Duman, S., Cakmak, Y., Kolemen, S., Akkaya, E. U. & Dede, Y.
Heavy Atom Free Singlet Oxygen Generation: Doubly Substituted
Configurations Dominate S1 States of Bis-BODIPYs. J. Org. Chem. 77,
13 Buyuktemiz, M., Duman, S. & Dede, Y. Luminescence of BODIPY
and Dipyrrin: An MCSCF Comparison of Excited States. J. Phys. Chem.
A 117, 1665-1669 (2013).
14 Gaussian 09 (Gaussian, Inc., Wallingford, CT, USA, 2009). 15
Vijay, D., Varathan, E. & Subramanian, V. Theoretical design of
core modified (oxa and thia) porphyrin based
organic dyes with bridging thiophene linkers. Journal of Materials
Chemistry A 1, 4358-4369, doi:10.1039/c3ta10270j (2013).